#------------------------------------------------------------------------------
#$Date: 2019-11-17 09:11:32 +0200 (Sun, 17 Nov 2019) $
#$Revision: 229032 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/07/7230703.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7230703
loop_
_publ_author_name
'Li, Feng-rui'
'Lv, Jing-hua'
'Yu, Kai'
'Zhang, Mao-lin'
'Wang, Kun-peng'
'Meng, Fan-xue'
'Zhou, Bai-bin'
_publ_section_title
;
 Effective photocatalytic and bifunctional electrocatalytic materials
 based on Keggin arsenomolybdates and different transition metal capped
 assemblies
;
_journal_issue                   25
_journal_name_full               CrystEngComm
_journal_page_first              3522
_journal_paper_doi               10.1039/C8CE00550H
_journal_volume                  20
_journal_year                    2018
_chemical_formula_moiety         'C30 H30 As Cu5 Mo12 N20 O42 V2'
_chemical_formula_sum            'C30 H30 As Cu5 Mo12 N20 O42 V2'
_chemical_formula_weight         2988.57
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2018-05-09 deposited with the CCDC.
2018-05-21 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 113.289(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   20.7262(6)
_cell_length_b                   14.6357(6)
_cell_length_c                   25.6626(9)
_cell_measurement_reflns_used    6345
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.08
_cell_measurement_theta_min      1.73
_cell_volume                     7150.3(5)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    SHELXP-97
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker Smart APEX CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0457
_diffrn_reflns_av_sigmaI/netI    0.0430
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_number            22949
_diffrn_reflns_theta_full        25.08
_diffrn_reflns_theta_max         25.08
_diffrn_reflns_theta_min         1.73
_exptl_absorpt_coefficient_mu    4.287
_exptl_absorpt_correction_T_max  0.501
_exptl_absorpt_correction_T_min  0.405
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    2.776
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             5656
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.16
_refine_diff_density_max         1.729
_refine_diff_density_min         -1.853
_refine_diff_density_rms         0.201
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.050
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     509
_refine_ls_number_reflns         6345
_refine_ls_number_restraints     18
_refine_ls_restrained_S_all      1.052
_refine_ls_R_factor_all          0.0639
_refine_ls_R_factor_gt           0.0484
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0610P)²+174.2442P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1351
_refine_ls_wR_factor_ref         0.1451
_reflns_number_gt                4944
_reflns_number_total             6345
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c8ce00550h2.cif
_cod_data_source_block           3
_cod_depositor_comments
'Adding full bibliography for 7230701--7230703.cif.'
_cod_original_cell_volume        7150.3(4)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               7230703
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
As1 As 0.5000 0.32037(9) 0.2500 0.0214(3) Uani 1 2 d S
C1 C 0.5643(6) 0.3069(7) 0.4916(5) 0.041(3) Uani 1 1 d .
H1 H 0.5655 0.3347 0.4594 0.049 Uiso 1 1 calc R
C2 C 0.5899(8) 0.2191(11) 0.5664(6) 0.081(5) Uani 1 1 d .
H2 H 0.6115 0.1768 0.5951 0.097 Uiso 1 1 calc R
C3 C 0.5341(8) 0.2697(11) 0.5592(6) 0.078(5) Uani 1 1 d .
H3 H 0.5092 0.2675 0.5825 0.093 Uiso 1 1 calc R
C4 C 0.3439(7) 0.5347(9) 0.4121(5) 0.058(4) Uani 1 1 d .
H4 H 0.3654 0.5328 0.3865 0.069 Uiso 1 1 calc R
C5 C 0.3213(6) 0.5111(9) 0.4844(5) 0.053(3) Uani 1 1 d .
H5 H 0.3239 0.4898 0.5193 0.063 Uiso 1 1 calc R
C6 C 0.2737(7) 0.5707(10) 0.4506(6) 0.068(4) Uani 1 1 d .
H6 H 0.2372 0.5968 0.4579 0.081 Uiso 1 1 calc R
C7 C 0.6534(10) 0.7546(15) 0.3910(11) 0.142(7) Uani 1 1 d U
H7 H 0.6370 0.7012 0.4012 0.171 Uiso 1 1 calc R
N5 N 0.7226(8) 0.8477(12) 0.3817(8) 0.110(5) Uani 1 1 d .
C9 C 0.6557(9) 0.8696(16) 0.3514(9) 0.111(7) Uani 1 1 d .
H9 H 0.6422 0.9194 0.3269 0.133 Uiso 1 1 calc R
C10 C 0.3700(7) 0.7560(11) 0.2909(6) 0.065(4) Uani 1 1 d .
H10 H 0.3803 0.6945 0.2895 0.077 Uiso 1 1 calc R
C11 C 0.3802(9) 0.9010(11) 0.3009(8) 0.083(5) Uani 1 1 d .
H11 H 0.3996 0.9593 0.3085 0.100 Uiso 1 1 calc R
N8 N 0.3124(8) 0.8821(13) 0.2829(9) 0.124(7) Uani 1 1 d .
C13 C 0.1143(8) 0.5785(14) 0.0914(9) 0.110(8) Uani 1 1 d .
H13 H 0.0855 0.6051 0.1072 0.132 Uiso 1 1 calc R
N9 N 0.1847(6) 0.5796(10) 0.1156(6) 0.089(5) Uani 1 1 d .
C15 C 0.1508(9) 0.5135(13) 0.0374(8) 0.093(6) Uani 1 1 d .
H15 H 0.1523 0.4844 0.0057 0.112 Uiso 1 1 calc R
V1 V 0.5000 0.04348(14) 0.2500 0.0217(5) Uani 1 2 d S
V2 V 0.5000 0.59787(13) 0.2500 0.0155(4) Uani 1 2 d S
Cu1 Cu 0.44388(9) 0.40983(11) 0.48625(7) 0.0581(5) Uani 1 1 d .
Cu2 Cu 0.51395(9) 0.82056(13) 0.32453(9) 0.0703(5) Uani 1 1 d .
Cu3 Cu 0.0000 0.5000 0.0000 0.1025(12) Uani 1 2 d S
Mo1 Mo 0.45792(4) 0.15389(5) 0.13791(3) 0.0229(2) Uani 1 1 d .
Mo2 Mo 0.36464(4) 0.15465(5) 0.22895(3) 0.02230(19) Uani 1 1 d .
Mo3 Mo 0.33499(5) 0.31379(6) 0.12555(4) 0.0322(2) Uani 1 1 d .
Mo4 Mo 0.36741(4) 0.48623(5) 0.23821(3) 0.02109(19) Uani 1 1 d .
Mo5 Mo 0.40497(5) 0.32738(6) 0.34144(4) 0.0342(2) Uani 1 1 d .
Mo6 Mo 0.52930(4) 0.48692(5) 0.36013(3) 0.02080(19) Uani 1 1 d .
N1 N 0.6097(6) 0.2422(8) 0.5223(4) 0.056(3) Uani 1 1 d .
N2 N 0.5180(5) 0.3254(7) 0.5133(4) 0.054(3) Uani 1 1 d .
N3 N 0.3652(5) 0.4874(6) 0.4588(4) 0.048(2) Uani 1 1 d .
N4 N 0.2879(6) 0.5858(7) 0.4049(4) 0.059(3) Uani 1 1 d .
C8 C 0.7196(10) 0.7738(15) 0.4076(11) 0.133(7) Uani 1 1 d U
H8 H 0.7572 0.7408 0.4330 0.160 Uiso 1 1 calc R
N6 N 0.6127(6) 0.8165(9) 0.3592(7) 0.085(4) Uani 1 1 d U
N7 N 0.4155(5) 0.8260(7) 0.3062(5) 0.052(3) Uani 1 1 d .
C12 C 0.3036(8) 0.7951(14) 0.2773(7) 0.099(7) Uani 1 1 d .
H12 H 0.2611 0.7640 0.2664 0.119 Uiso 1 1 calc R
C14 C 0.2062(8) 0.5379(12) 0.0821(7) 0.086(5) Uani 1 1 d .
H14 H 0.2528 0.5266 0.0882 0.103 Uiso 1 1 calc R
N10 N 0.0918(6) 0.5363(9) 0.0438(5) 0.073(4) Uani 1 1 d .
O1 O 0.5000 -0.0655(7) 0.2500 0.043(3) Uani 1 2 d S
O2 O 0.4139(3) 0.0861(4) 0.1852(3) 0.0252(14) Uani 1 1 d .
O3 O 0.5426(3) 0.1118(4) 0.2087(3) 0.0243(13) Uani 1 1 d .
O4 O 0.4584(4) 0.0709(5) 0.0926(3) 0.0353(16) Uani 1 1 d .
O5 O 0.5173(3) 0.2412(4) 0.1315(2) 0.0258(14) Uani 1 1 d .
O6 O 0.3758(3) 0.2143(4) 0.0964(2) 0.0258(14) Uani 1 1 d .
O7 O 0.4379(3) 0.2558(4) 0.2033(2) 0.0200(12) Uani 1 1 d .
O8 O 0.3101(3) 0.0732(4) 0.2330(3) 0.0346(16) Uani 1 1 d .
O9 O 0.3059(3) 0.2156(4) 0.1639(2) 0.0235(13) Uani 1 1 d .
O10 O 0.2614(3) 0.3328(5) 0.0700(3) 0.0356(16) Uani 1 1 d .
O11 O 0.4016(3) 0.3998(4) 0.1164(2) 0.0221(13) Uani 1 1 d .
O12 O 0.3624(3) 0.2410(4) 0.2791(2) 0.0239(13) Uani 1 1 d .
O13 O 0.4638(3) 0.3847(4) 0.2845(2) 0.0171(12) Uani 1 1 d .
O14 O 0.3316(3) 0.3998(4) 0.1826(2) 0.0232(13) Uani 1 1 d .
O15 O 0.3473(3) 0.4264(4) 0.2929(2) 0.0233(13) Uani 1 1 d .
O16 O 0.4678(3) 0.4267(4) 0.3838(2) 0.0223(13) Uani 1 1 d .
O17 O 0.3621(4) 0.3059(5) 0.3821(3) 0.0369(17) Uani 1 1 d .
O18 O 0.5593(3) 0.5715(4) 0.4082(3) 0.0283(14) Uani 1 1 d .
O19 O 0.4499(3) 0.5551(4) 0.2981(2) 0.0217(13) Uani 1 1 d .
O20 O 0.5722(3) 0.5276(4) 0.3048(2) 0.0223(13) Uani 1 1 d .
O21 O 0.3069(3) 0.5694(4) 0.2184(3) 0.0291(14) Uani 1 1 d .
O22 O 0.5000 0.7070(7) 0.2500 0.047(3) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O13 As1 O13 110.9(4) . 2_655
O13 As1 O7 108.8(3) . 2_655
O13 As1 O7 108.8(3) 2_655 2_655
O13 As1 O7 108.8(3) . .
O13 As1 O7 108.8(3) 2_655 .
O7 As1 O7 110.8(4) 2_655 .
N2 C1 N1 110.8(10) . .
N2 C1 H1 124.6 . .
N1 C1 H1 124.6 . .
C3 C2 N1 105.9(11) . .
C3 C2 H2 127.1 . .
N1 C2 H2 127.1 . .
C2 C3 N2 110.9(11) . .
C2 C3 H3 124.5 . .
N2 C3 H3 124.5 . .
N3 C4 N4 112.7(12) . .
N3 C4 H4 123.6 . .
N4 C4 H4 123.6 . .
C6 C5 N3 108.4(12) . .
C6 C5 H5 125.8 . .
N3 C5 H5 125.8 . .
N4 C6 C5 108.2(12) . .
N4 C6 H6 125.9 . .
C5 C6 H6 125.9 . .
N6 C7 C8 113(2) . .
N6 C7 H7 123.3 . .
C8 C7 H7 123.3 . .
C8 N5 C9 104.6(16) . .
N6 C9 N5 113.5(19) . .
N6 C9 H9 123.3 . .
N5 C9 H9 123.3 . .
N7 C10 C12 105.6(14) . .
N7 C10 H10 127.2 . .
C12 C10 H10 127.2 . .
N7 C11 N8 109.7(16) . .
N7 C11 H11 125.2 . .
N8 C11 H11 125.2 . .
C12 N8 C11 109.3(15) . .
N10 C13 N9 111.7(14) . .
N10 C13 H13 124.2 . .
N9 C13 H13 124.2 . .
C14 N9 C13 106.7(13) . .
C14 C15 N10 110.5(14) . .
C14 C15 H15 124.7 . .
N10 C15 H15 124.7 . .
O1 V1 O3 121.58(19) . 2_655
O1 V1 O3 121.58(18) . .
O3 V1 O3 116.8(4) 2_655 .
O1 V1 O2 108.21(18) . 2_655
O3 V1 O2 80.3(2) 2_655 2_655
O3 V1 O2 80.9(2) . 2_655
O1 V1 O2 108.21(18) . .
O3 V1 O2 80.9(2) 2_655 .
O3 V1 O2 80.3(2) . .
O2 V1 O2 143.6(4) 2_655 .
O1 V1 Mo2 121.66(4) . .
O3 V1 Mo2 40.21(18) 2_655 .
O3 V1 Mo2 102.36(19) . .
O2 V1 Mo2 115.47(18) 2_655 .
O2 V1 Mo2 40.71(17) . .
O1 V1 Mo2 121.66(4) . 2_655
O3 V1 Mo2 102.36(19) 2_655 2_655
O3 V1 Mo2 40.21(18) . 2_655
O2 V1 Mo2 40.71(17) 2_655 2_655
O2 V1 Mo2 115.47(18) . 2_655
Mo2 V1 Mo2 116.69(7) . 2_655
O1 V1 Mo1 121.32(4) . 2_655
O3 V1 Mo1 40.19(18) 2_655 2_655
O3 V1 Mo1 102.68(19) . 2_655
O2 V1 Mo1 40.20(17) 2_655 2_655
O2 V1 Mo1 116.04(18) . 2_655
Mo2 V1 Mo1 77.99(4) . 2_655
Mo2 V1 Mo1 70.27(3) 2_655 2_655
O1 V1 Mo1 121.32(4) . .
O3 V1 Mo1 102.68(19) 2_655 .
O3 V1 Mo1 40.19(18) . .
O2 V1 Mo1 116.04(18) 2_655 .
O2 V1 Mo1 40.20(17) . .
Mo2 V1 Mo1 70.27(3) . .
Mo2 V1 Mo1 77.99(4) 2_655 .
Mo1 V1 Mo1 117.35(7) 2_655 .
O22 V2 O20 122.78(18) . 2_655
O22 V2 O20 122.78(18) . .
O20 V2 O20 114.4(4) 2_655 .
O22 V2 O19 108.21(17) . 2_655
O20 V2 O19 79.8(2) 2_655 2_655
O20 V2 O19 80.7(2) . 2_655
O22 V2 O19 108.21(17) . .
O20 V2 O19 80.7(2) 2_655 .
O20 V2 O19 79.8(2) . .
O19 V2 O19 143.6(3) 2_655 .
O22 V2 Mo6 121.54(3) . 2_655
O20 V2 Mo6 39.62(17) 2_655 2_655
O20 V2 Mo6 101.76(18) . 2_655
O19 V2 Mo6 40.34(16) 2_655 2_655
O19 V2 Mo6 115.80(17) . 2_655
O22 V2 Mo4 121.72(3) . .
O20 V2 Mo4 40.17(17) 2_655 .
O20 V2 Mo4 101.23(18) . .
O19 V2 Mo4 115.48(18) 2_655 .
O19 V2 Mo4 40.63(16) . .
Mo6 V2 Mo4 77.83(4) 2_655 .
O22 V2 Mo4 121.72(3) . 2_655
O20 V2 Mo4 101.23(18) 2_655 2_655
O20 V2 Mo4 40.17(17) . 2_655
O19 V2 Mo4 40.63(16) 2_655 2_655
O19 V2 Mo4 115.48(18) . 2_655
Mo6 V2 Mo4 70.17(3) 2_655 2_655
Mo4 V2 Mo4 116.55(7) . 2_655
N2 Cu1 N3 175.8(5) . .
N6 Cu2 N7 167.4(6) . .
N10 Cu3 N10 179.997(1) . 5_565
O4 Mo1 O5 104.8(3) . .
O4 Mo1 O6 101.8(3) . .
O5 Mo1 O6 96.6(3) . .
O4 Mo1 O2 100.7(3) . .
O5 Mo1 O2 150.4(3) . .
O6 Mo1 O2 92.8(3) . .
O4 Mo1 O3 99.0(3) . .
O5 Mo1 O3 85.3(3) . .
O6 Mo1 O3 157.9(2) . .
O2 Mo1 O3 75.8(2) . .
O4 Mo1 O7 168.6(3) . .
O5 Mo1 O7 86.4(2) . .
O6 Mo1 O7 74.3(2) . .
O2 Mo1 O7 69.2(2) . .
O3 Mo1 O7 83.8(2) . .
O4 Mo1 V1 100.8(2) . .
O5 Mo1 V1 119.63(19) . .
O6 Mo1 V1 130.01(19) . .
O2 Mo1 V1 39.18(17) . .
O3 Mo1 V1 36.74(16) . .
O7 Mo1 V1 74.88(14) . .
O8 Mo2 O12 104.2(3) . .
O8 Mo2 O9 100.3(3) . .
O12 Mo2 O9 96.4(3) . .
O8 Mo2 O2 100.4(3) . .
O12 Mo2 O2 152.1(2) . .
O9 Mo2 O2 91.9(3) . .
O8 Mo2 O3 100.4(3) . 2_655
O12 Mo2 O3 86.5(3) . 2_655
O9 Mo2 O3 157.7(2) . 2_655
O2 Mo2 O3 76.2(2) . 2_655
O8 Mo2 O7 167.3(3) . .
O12 Mo2 O7 87.7(2) . .
O9 Mo2 O7 73.6(2) . .
O2 Mo2 O7 69.2(2) . .
O3 Mo2 O7 84.4(2) 2_655 .
O8 Mo2 V1 101.7(2) . .
O12 Mo2 V1 121.07(19) . .
O9 Mo2 V1 129.33(18) . .
O2 Mo2 V1 39.41(17) . .
O3 Mo2 V1 36.87(16) 2_655 .
O7 Mo2 V1 75.15(14) . .
O10 Mo3 O11 104.2(3) . .
O10 Mo3 O14 104.1(3) . .
O11 Mo3 O14 84.9(2) . .
O10 Mo3 O9 101.2(3) . .
O11 Mo3 O9 154.7(2) . .
O14 Mo3 O9 89.3(2) . .
O10 Mo3 O6 100.7(3) . .
O11 Mo3 O6 90.1(2) . .
O14 Mo3 O6 155.1(3) . .
O9 Mo3 O6 84.9(3) . .
O10 Mo3 O7 169.2(3) . .
O11 Mo3 O7 83.7(2) . .
O14 Mo3 O7 83.7(2) . .
O9 Mo3 O7 71.1(2) . .
O6 Mo3 O7 71.6(2) . .
O21 Mo4 O14 103.9(3) . .
O21 Mo4 O15 102.1(3) . .
O14 Mo4 O15 96.9(3) . .
O21 Mo4 O19 99.9(3) . .
O14 Mo4 O19 152.0(2) . .
O15 Mo4 O19 92.1(2) . .
O21 Mo4 O20 99.5(3) . 2_655
O14 Mo4 O20 86.0(2) . 2_655
O15 Mo4 O20 156.8(2) . 2_655
O19 Mo4 O20 75.8(2) . 2_655
O21 Mo4 O13 168.2(3) . .
O14 Mo4 O13 87.7(2) . .
O15 Mo4 O13 73.9(2) . .
O19 Mo4 O13 69.5(2) . .
O20 Mo4 O13 83.3(2) 2_655 .
O21 Mo4 V2 100.1(2) . .
O14 Mo4 V2 120.66(17) . .
O15 Mo4 V2 129.48(19) . .
O19 Mo4 V2 39.39(16) . .
O20 Mo4 V2 36.49(16) 2_655 .
O13 Mo4 V2 75.25(14) . .
O17 Mo5 O5 103.2(3) . 2_655
O17 Mo5 O12 102.3(3) . .
O5 Mo5 O12 85.1(3) 2_655 .
O17 Mo5 O16 101.3(3) . .
O5 Mo5 O16 90.5(3) 2_655 .
O12 Mo5 O16 156.3(2) . .
O17 Mo5 O15 101.3(3) . .
O5 Mo5 O15 155.5(2) 2_655 .
O12 Mo5 O15 89.6(3) . .
O16 Mo5 O15 84.9(2) . .
O17 Mo5 O13 170.5(3) . .
O5 Mo5 O13 84.0(2) 2_655 .
O12 Mo5 O13 84.3(2) . .
O16 Mo5 O13 72.2(2) . .
O15 Mo5 O13 71.7(2) . .
O18 Mo6 O11 104.9(3) . 2_655
O18 Mo6 O16 102.3(3) . .
O11 Mo6 O16 96.4(3) 2_655 .
O18 Mo6 O20 99.2(3) . .
O11 Mo6 O20 86.1(2) 2_655 .
O16 Mo6 O20 156.9(2) . .
O18 Mo6 O19 99.3(3) . .
O11 Mo6 O19 151.7(2) 2_655 .
O16 Mo6 O19 92.4(2) . .
O20 Mo6 O19 75.7(2) . .
O18 Mo6 O13 167.8(3) . .
O11 Mo6 O13 87.2(2) 2_655 .
O16 Mo6 O13 74.0(2) . .
O20 Mo6 O13 83.2(2) . .
O19 Mo6 O13 69.5(2) . .
C1 N1 C2 106.6(10) . .
C1 N2 C3 105.9(10) . .
C1 N2 Cu1 127.3(8) . .
C3 N2 Cu1 126.8(8) . .
C4 N3 C5 105.2(10) . .
C4 N3 Cu1 126.4(9) . .
C5 N3 Cu1 128.3(8) . .
C4 N4 C6 105.5(10) . .
N5 C8 C7 106.0(19) . .
N5 C8 H8 127.0 . .
C7 C8 H8 127.0 . .
C9 N6 C7 102.0(15) . .
C9 N6 Cu2 127.8(13) . .
C7 N6 Cu2 129.8(13) . .
C11 N7 C10 108.3(13) . .
C11 N7 Cu2 124.4(10) . .
C10 N7 Cu2 127.0(9) . .
N8 C12 C10 107.0(13) . .
N8 C12 H12 126.5 . .
C10 C12 H12 126.5 . .
N9 C14 C15 107.7(14) . .
N9 C14 H14 126.2 . .
C15 C14 H14 126.2 . .
C13 N10 C15 103.3(13) . .
C13 N10 Cu3 127.9(12) . .
C15 N10 Cu3 128.2(11) . .
V1 O2 Mo1 100.6(3) . .
V1 O2 Mo2 99.9(3) . .
Mo1 O2 Mo2 121.6(3) . .
V1 O3 Mo2 102.9(3) . 2_655
V1 O3 Mo1 103.1(3) . .
Mo2 O3 Mo1 143.6(3) 2_655 .
Mo1 O5 Mo5 156.1(3) . 2_655
Mo1 O6 Mo3 125.0(3) . .
As1 O7 Mo2 123.2(3) . .
As1 O7 Mo1 123.9(3) . .
Mo2 O7 Mo1 96.4(2) . .
As1 O7 Mo3 124.9(3) . .
Mo2 O7 Mo3 89.75(19) . .
Mo1 O7 Mo3 88.94(19) . .
Mo2 O9 Mo3 125.4(3) . .
Mo6 O11 Mo3 155.3(3) 2_655 .
Mo2 O12 Mo5 154.2(3) . .
As1 O13 Mo4 123.5(3) . .
As1 O13 Mo5 125.0(3) . .
Mo4 O13 Mo5 89.61(18) . .
As1 O13 Mo6 123.7(3) . .
Mo4 O13 Mo6 96.2(2) . .
Mo5 O13 Mo6 89.20(17) . .
Mo4 O14 Mo3 155.0(3) . .
Mo4 O15 Mo5 124.6(3) . .
Mo6 O16 Mo5 124.4(3) . .
V2 O19 Mo6 100.3(3) . .
V2 O19 Mo4 100.0(2) . .
Mo6 O19 Mo4 121.3(3) . .
V2 O20 Mo6 104.0(3) . .
V2 O20 Mo4 103.3(3) . 2_655
Mo6 O20 Mo4 144.2(3) . 2_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
As1 O13 1.660(5) .
As1 O13 1.660(5) 2_655
As1 O7 1.664(6) 2_655
As1 O7 1.664(6) .
C1 N2 1.315(14) .
C1 N1 1.347(14) .
C1 H1 0.9300 .
C2 C3 1.323(18) .
C2 N1 1.390(16) .
C2 H2 0.9300 .
C3 N2 1.361(15) .
C3 H3 0.9300 .
C4 N3 1.302(15) .
C4 N4 1.331(15) .
C4 H4 0.9300 .
C5 C6 1.345(17) .
C5 N3 1.358(15) .
C5 H5 0.9300 .
C6 N4 1.338(18) .
C6 H6 0.9300 .
C7 N6 1.29(2) .
C7 C8 1.30(2) .
C7 H7 0.9300 .
N5 C8 1.28(2) .
N5 C9 1.33(2) .
C9 N6 1.26(2) .
C9 H9 0.9300 .
C10 N7 1.341(16) .
C10 C12 1.40(2) .
C10 H10 0.9300 .
C11 N7 1.297(17) .
C11 N8 1.32(2) .
C11 H11 0.9300 .
N8 C12 1.29(2) .
C13 N10 1.279(19) .
C13 N9 1.341(18) .
C13 H13 0.9300 .
N9 C14 1.270(19) .
C15 C14 1.31(2) .
C15 N10 1.340(19) .
C15 H15 0.9300 .
V1 O1 1.596(11) .
V1 O3 1.909(6) 2_655
V1 O3 1.909(6) .
V1 O2 1.998(6) 2_655
V1 O2 1.998(6) .
V1 Mo2 3.1002(13) .
V1 Mo2 3.1003(13) 2_655
V1 Mo1 3.1083(13) 2_655
V1 Mo1 3.1084(13) .
V2 O22 1.598(11) .
V2 O20 1.899(6) 2_655
V2 O20 1.899(6) .
V2 O19 2.002(6) 2_655
V2 O19 2.002(6) .
V2 Mo6 3.1042(13) 2_655
V2 Mo4 3.1073(13) .
V2 Mo4 3.1074(13) 2_655
Cu1 N2 1.878(9) .
Cu1 N3 1.881(9) .
Cu2 N6 1.882(11) .
Cu2 N7 1.906(10) .
Cu3 N10 1.864(11) .
Cu3 N10 1.864(11) 5_565
Mo1 O4 1.684(6) .
Mo1 O5 1.826(6) .
Mo1 O6 1.837(6) .
Mo1 O2 2.041(6) .
Mo1 O3 2.059(6) .
Mo1 O7 2.400(6) .
Mo2 O8 1.673(6) .
Mo2 O12 1.816(6) .
Mo2 O9 1.860(6) .
Mo2 O2 2.052(6) .
Mo2 O3 2.053(6) 2_655
Mo2 O7 2.392(5) .
Mo3 O10 1.648(7) .
Mo3 O11 1.950(6) .
Mo3 O14 1.953(6) .
Mo3 O9 1.966(6) .
Mo3 O6 1.974(6) .
Mo3 O7 2.426(6) .
Mo4 O21 1.677(6) .
Mo4 O14 1.831(6) .
Mo4 O15 1.836(6) .
Mo4 O19 2.055(6) .
Mo4 O20 2.060(6) 2_655
Mo4 O13 2.395(5) .
Mo5 O17 1.645(6) .
Mo5 O5 1.945(6) 2_655
Mo5 O12 1.955(6) .
Mo5 O16 1.968(6) .
Mo5 O15 1.976(6) .
Mo5 O13 2.396(5) .
Mo6 O18 1.684(6) .
Mo6 O11 1.832(6) 2_655
Mo6 O16 1.840(6) .
Mo6 O20 2.040(6) .
Mo6 O19 2.042(6) .
Mo6 O13 2.401(5) .
C8 H8 0.9300 .
C12 H12 0.9300 .
C14 H14 0.9300 .
O3 Mo2 2.053(6) 2_655
O5 Mo5 1.945(6) 2_655
O11 Mo6 1.832(6) 2_655
O20 Mo4 2.060(6) 2_655
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
N1 C2 C3 N2 -1(2) . .
N3 C5 C6 N4 -1.1(16) . .
C8 N5 C9 N6 3(3) . .
N7 C11 N8 C12 1(2) . .
N10 C13 N9 C14 1(3) . .
O1 V1 Mo1 O4 -12.6(2) . .
O3 V1 Mo1 O4 -152.5(3) 2_655 .
O3 V1 Mo1 O4 90.7(4) . .
O2 V1 Mo1 O4 122.2(3) 2_655 .
O2 V1 Mo1 O4 -93.7(4) . .
Mo2 V1 Mo1 O4 -128.3(2) . .
Mo2 V1 Mo1 O4 107.3(2) 2_655 .
Mo1 V1 Mo1 O4 167.4(2) 2_655 .
O1 V1 Mo1 O5 -126.6(2) . .
O3 V1 Mo1 O5 93.5(3) 2_655 .
O3 V1 Mo1 O5 -23.3(4) . .
O2 V1 Mo1 O5 8.2(3) 2_655 .
O2 V1 Mo1 O5 152.2(3) . .
Mo2 V1 Mo1 O5 117.7(2) . .
Mo2 V1 Mo1 O5 -6.7(2) 2_655 .
Mo1 V1 Mo1 O5 53.4(2) 2_655 .
O1 V1 Mo1 O6 103.0(2) . .
O3 V1 Mo1 O6 -37.0(3) 2_655 .
O3 V1 Mo1 O6 -153.8(4) . .
O2 V1 Mo1 O6 -122.3(3) 2_655 .
O2 V1 Mo1 O6 21.8(4) . .
Mo2 V1 Mo1 O6 -12.8(2) . .
Mo2 V1 Mo1 O6 -137.1(2) 2_655 .
Mo1 V1 Mo1 O6 -77.0(2) 2_655 .
O1 V1 Mo1 O2 81.2(3) . .
O3 V1 Mo1 O2 -58.8(3) 2_655 .
O3 V1 Mo1 O2 -175.6(4) . .
O2 V1 Mo1 O2 -144.1(4) 2_655 .
Mo2 V1 Mo1 O2 -34.6(3) . .
Mo2 V1 Mo1 O2 -158.9(3) 2_655 .
Mo1 V1 Mo1 O2 -98.8(3) 2_655 .
O1 V1 Mo1 O3 -103.3(3) . .
O3 V1 Mo1 O3 116.8(4) 2_655 .
O2 V1 Mo1 O3 31.5(3) 2_655 .
O2 V1 Mo1 O3 175.6(4) . .
Mo2 V1 Mo1 O3 141.0(3) . .
Mo2 V1 Mo1 O3 16.6(3) 2_655 .
Mo1 V1 Mo1 O3 76.7(3) 2_655 .
O1 V1 Mo1 O7 156.62(13) . .
O3 V1 Mo1 O7 16.7(2) 2_655 .
O3 V1 Mo1 O7 -100.1(3) . .
O2 V1 Mo1 O7 -68.6(2) 2_655 .
O2 V1 Mo1 O7 75.5(3) . .
Mo2 V1 Mo1 O7 40.88(14) . .
Mo2 V1 Mo1 O7 -83.46(14) 2_655 .
Mo1 V1 Mo1 O7 -23.37(13) 2_655 .
O1 V1 Mo2 O8 11.0(2) . .
O3 V1 Mo2 O8 -91.9(4) 2_655 .
O3 V1 Mo2 O8 150.9(3) . .
O2 V1 Mo2 O8 -123.4(3) 2_655 .
O2 V1 Mo2 O8 92.2(4) . .
Mo2 V1 Mo2 O8 -169.0(2) 2_655 .
Mo1 V1 Mo2 O8 -108.5(2) 2_655 .
Mo1 V1 Mo2 O8 126.4(2) . .
O1 V1 Mo2 O12 125.7(2) . .
O3 V1 Mo2 O12 22.7(4) 2_655 .
O3 V1 Mo2 O12 -94.4(3) . .
O2 V1 Mo2 O12 -8.8(3) 2_655 .
O2 V1 Mo2 O12 -153.2(3) . .
Mo2 V1 Mo2 O12 -54.3(2) 2_655 .
Mo1 V1 Mo2 O12 6.1(2) 2_655 .
Mo1 V1 Mo2 O12 -119.0(2) . .
O1 V1 Mo2 O9 -102.9(2) . .
O3 V1 Mo2 O9 154.2(4) 2_655 .
O3 V1 Mo2 O9 37.0(3) . .
O2 V1 Mo2 O9 122.7(3) 2_655 .
O2 V1 Mo2 O9 -21.7(4) . .
Mo2 V1 Mo2 O9 77.1(2) 2_655 .
Mo1 V1 Mo2 O9 137.6(2) 2_655 .
Mo1 V1 Mo2 O9 12.4(2) . .
O1 V1 Mo2 O2 -81.1(3) . .
O3 V1 Mo2 O2 175.9(4) 2_655 .
O3 V1 Mo2 O2 58.7(3) . .
O2 V1 Mo2 O2 144.4(4) 2_655 .
Mo2 V1 Mo2 O2 98.8(3) 2_655 .
Mo1 V1 Mo2 O2 159.3(3) 2_655 .
Mo1 V1 Mo2 O2 34.2(3) . .
O1 V1 Mo2 O3 102.9(3) . 2_655
O3 V1 Mo2 O3 -117.2(4) . 2_655
O2 V1 Mo2 O3 -31.5(3) 2_655 2_655
O2 V1 Mo2 O3 -175.9(4) . 2_655
Mo2 V1 Mo2 O3 -77.1(3) 2_655 2_655
Mo1 V1 Mo2 O3 -16.6(3) 2_655 2_655
Mo1 V1 Mo2 O3 -141.8(3) . 2_655
O1 V1 Mo2 O7 -156.32(14) . .
O3 V1 Mo2 O7 100.8(3) 2_655 .
O3 V1 Mo2 O7 -16.4(2) . .
O2 V1 Mo2 O7 69.2(2) 2_655 .
O2 V1 Mo2 O7 -75.2(3) . .
Mo2 V1 Mo2 O7 23.68(14) 2_655 .
Mo1 V1 Mo2 O7 84.13(14) 2_655 .
Mo1 V1 Mo2 O7 -41.00(14) . .
O22 V2 Mo4 O21 12.4(2) . .
O20 V2 Mo4 O21 -92.3(3) 2_655 .
O20 V2 Mo4 O21 152.9(3) . .
O19 V2 Mo4 O21 -122.2(3) 2_655 .
O19 V2 Mo4 O21 93.4(3) . .
Mo6 V2 Mo4 O21 -107.3(2) 2_655 .
Mo4 V2 Mo4 O21 -167.6(2) 2_655 .
O22 V2 Mo4 O14 125.3(2) . .
O20 V2 Mo4 O14 20.6(4) 2_655 .
O20 V2 Mo4 O14 -94.2(3) . .
O19 V2 Mo4 O14 -9.2(3) 2_655 .
O19 V2 Mo4 O14 -153.7(3) . .
Mo6 V2 Mo4 O14 5.6(2) 2_655 .
Mo4 V2 Mo4 O14 -54.7(2) 2_655 .
O22 V2 Mo4 O15 -102.6(2) . .
O20 V2 Mo4 O15 152.7(4) 2_655 .
O20 V2 Mo4 O15 37.9(3) . .
O19 V2 Mo4 O15 122.9(3) 2_655 .
O19 V2 Mo4 O15 -21.6(3) . .
Mo6 V2 Mo4 O15 137.7(2) 2_655 .
Mo4 V2 Mo4 O15 77.4(2) 2_655 .
O22 V2 Mo4 O19 -81.0(3) . .
O20 V2 Mo4 O19 174.2(4) 2_655 .
O20 V2 Mo4 O19 59.5(3) . .
O19 V2 Mo4 O19 144.4(3) 2_655 .
Mo6 V2 Mo4 O19 159.3(3) 2_655 .
Mo4 V2 Mo4 O19 99.0(3) 2_655 .
O22 V2 Mo4 O20 104.7(3) . 2_655
O20 V2 Mo4 O20 -114.7(4) . 2_655
O19 V2 Mo4 O20 -29.8(3) 2_655 2_655
O19 V2 Mo4 O20 -174.2(4) . 2_655
Mo6 V2 Mo4 O20 -15.0(3) 2_655 2_655
Mo4 V2 Mo4 O20 -75.3(3) 2_655 2_655
O22 V2 Mo4 O13 -156.50(13) . .
O20 V2 Mo4 O13 98.8(3) 2_655 .
O20 V2 Mo4 O13 -16.0(2) . .
O19 V2 Mo4 O13 68.9(2) 2_655 .
O19 V2 Mo4 O13 -75.5(3) . .
Mo6 V2 Mo4 O13 83.78(13) 2_655 .
Mo4 V2 Mo4 O13 23.50(13) 2_655 .
N2 C1 N1 C2 -0.1(16) . .
C3 C2 N1 C1 0.8(19) . .
N1 C1 N2 C3 -0.6(16) . .
N1 C1 N2 Cu1 -179.8(9) . .
C2 C3 N2 C1 1(2) . .
C2 C3 N2 Cu1 -179.7(12) . .
N3 Cu1 N2 C1 123(5) . .
N3 Cu1 N2 C3 -56(6) . .
N4 C4 N3 C5 -1.6(16) . .
N4 C4 N3 Cu1 -177.8(9) . .
C6 C5 N3 C4 1.7(15) . .
C6 C5 N3 Cu1 177.7(9) . .
N2 Cu1 N3 C4 -119(6) . .
N2 Cu1 N3 C5 65(6) . .
N3 C4 N4 C6 0.9(16) . .
C5 C6 N4 C4 0.2(16) . .
C9 N5 C8 C7 1(3) . .
N6 C7 C8 N5 -5(4) . .
N5 C9 N6 C7 -6(3) . .
N5 C9 N6 Cu2 -178.9(14) . .
C8 C7 N6 C9 7(3) . .
C8 C7 N6 Cu2 179.7(19) . .
N7 Cu2 N6 C9 -123(3) . .
N7 Cu2 N6 C7 66(4) . .
N8 C11 N7 C10 0.6(19) . .
N8 C11 N7 Cu2 174.3(12) . .
C12 C10 N7 C11 -1.8(17) . .
C12 C10 N7 Cu2 -175.2(10) . .
N6 Cu2 N7 C11 86(3) . .
N6 Cu2 N7 C10 -102(3) . .
C11 N8 C12 C10 -2(2) . .
N7 C10 C12 N8 2(2) . .
C13 N9 C14 C15 2(2) . .
N10 C15 C14 N9 -3(2) . .
N9 C13 N10 C15 -2(2) . .
N9 C13 N10 Cu3 169.2(13) . .
C14 C15 N10 C13 3(2) . .
C14 C15 N10 Cu3 -168.1(14) . .
N10 Cu3 N10 C13 26(4) 5_565 .
N10 Cu3 N10 C15 -164(4) 5_565 .
O1 V1 O2 Mo1 -117.30(19) . .
O3 V1 O2 Mo1 122.3(3) 2_655 .
O3 V1 O2 Mo1 2.9(3) . .
O2 V1 O2 Mo1 62.70(18) 2_655 .
Mo2 V1 O2 Mo1 125.0(4) . .
Mo2 V1 O2 Mo1 22.9(3) 2_655 .
Mo1 V1 O2 Mo1 102.4(2) 2_655 .
O1 V1 O2 Mo2 117.70(18) . .
O3 V1 O2 Mo2 -2.7(2) 2_655 .
O3 V1 O2 Mo2 -122.1(3) . .
O2 V1 O2 Mo2 -62.30(18) 2_655 .
Mo2 V1 O2 Mo2 -102.1(2) 2_655 .
Mo1 V1 O2 Mo2 -22.6(3) 2_655 .
Mo1 V1 O2 Mo2 -125.0(4) . .
O4 Mo1 O2 V1 94.0(3) . .
O5 Mo1 O2 V1 -54.9(6) . .
O6 Mo1 O2 V1 -163.5(3) . .
O3 Mo1 O2 V1 -2.7(2) . .
O7 Mo1 O2 V1 -91.4(3) . .
O4 Mo1 O2 Mo2 -157.3(4) . .
O5 Mo1 O2 Mo2 53.7(7) . .
O6 Mo1 O2 Mo2 -54.8(4) . .
O3 Mo1 O2 Mo2 106.0(4) . .
O7 Mo1 O2 Mo2 17.3(3) . .
V1 Mo1 O2 Mo2 108.7(4) . .
O8 Mo2 O2 V1 -95.8(3) . .
O12 Mo2 O2 V1 55.7(6) . .
O9 Mo2 O2 V1 163.3(3) . .
O3 Mo2 O2 V1 2.5(2) 2_655 .
O7 Mo2 O2 V1 91.7(3) . .
O8 Mo2 O2 Mo1 155.1(4) . .
O12 Mo2 O2 Mo1 -53.3(7) . .
O9 Mo2 O2 Mo1 54.3(4) . .
O3 Mo2 O2 Mo1 -106.6(4) 2_655 .
O7 Mo2 O2 Mo1 -17.3(3) . .
V1 Mo2 O2 Mo1 -109.1(4) . .
O1 V1 O3 Mo2 -103.1(2) . 2_655
O3 V1 O3 Mo2 76.9(2) 2_655 2_655
O2 V1 O3 Mo2 2.7(3) 2_655 2_655
O2 V1 O3 Mo2 151.4(3) . 2_655
Mo2 V1 O3 Mo2 116.9(2) . 2_655
Mo1 V1 O3 Mo2 36.7(2) 2_655 2_655
Mo1 V1 O3 Mo2 154.3(4) . 2_655
O1 V1 O3 Mo1 102.6(2) . .
O3 V1 O3 Mo1 -77.4(2) 2_655 .
O2 V1 O3 Mo1 -151.6(3) 2_655 .
O2 V1 O3 Mo1 -2.9(3) . .
Mo2 V1 O3 Mo1 -37.3(2) . .
Mo2 V1 O3 Mo1 -154.3(4) 2_655 .
Mo1 V1 O3 Mo1 -117.6(2) 2_655 .
O4 Mo1 O3 V1 -95.9(3) . .
O5 Mo1 O3 V1 159.8(3) . .
O6 Mo1 O3 V1 63.9(8) . .
O2 Mo1 O3 V1 2.9(3) . .
O7 Mo1 O3 V1 72.9(3) . .
O4 Mo1 O3 Mo2 129.5(5) . 2_655
O5 Mo1 O3 Mo2 25.2(5) . 2_655
O6 Mo1 O3 Mo2 -70.7(9) . 2_655
O2 Mo1 O3 Mo2 -131.7(5) . 2_655
O7 Mo1 O3 Mo2 -61.6(5) . 2_655
V1 Mo1 O3 Mo2 -134.6(7) . 2_655
O4 Mo1 O5 Mo5 -129.9(9) . 2_655
O6 Mo1 O5 Mo5 126.1(9) . 2_655
O2 Mo1 O5 Mo5 18.5(13) . 2_655
O3 Mo1 O5 Mo5 -31.8(9) . 2_655
O7 Mo1 O5 Mo5 52.3(9) . 2_655
V1 Mo1 O5 Mo5 -18.0(10) . 2_655
O4 Mo1 O6 Mo3 173.4(4) . .
O5 Mo1 O6 Mo3 -79.9(4) . .
O2 Mo1 O6 Mo3 71.9(4) . .
O3 Mo1 O6 Mo3 13.8(9) . .
O7 Mo1 O6 Mo3 4.4(3) . .
V1 Mo1 O6 Mo3 58.3(5) . .
O10 Mo3 O6 Mo1 -176.7(4) . .
O11 Mo3 O6 Mo1 78.9(4) . .
O14 Mo3 O6 Mo1 1.0(8) . .
O9 Mo3 O6 Mo1 -76.2(4) . .
O7 Mo3 O6 Mo1 -4.5(3) . .
O13 As1 O7 Mo2 -56.1(4) . .
O13 As1 O7 Mo2 -177.0(3) 2_655 .
O7 As1 O7 Mo2 63.4(3) 2_655 .
O13 As1 O7 Mo1 176.9(3) . .
O13 As1 O7 Mo1 56.0(4) 2_655 .
O7 As1 O7 Mo1 -63.5(3) 2_655 .
O13 As1 O7 Mo3 60.7(4) . .
O13 As1 O7 Mo3 -60.2(4) 2_655 .
O7 As1 O7 Mo3 -179.8(4) 2_655 .
O8 Mo2 O7 As1 -161.5(11) . .
O12 Mo2 O7 As1 38.4(4) . .
O9 Mo2 O7 As1 135.8(4) . .
O2 Mo2 O7 As1 -125.6(4) . .
O3 Mo2 O7 As1 -48.3(4) 2_655 .
V1 Mo2 O7 As1 -84.6(3) . .
O8 Mo2 O7 Mo1 -23.4(13) . .
O12 Mo2 O7 Mo1 176.6(2) . .
O9 Mo2 O7 Mo1 -86.1(2) . .
O2 Mo2 O7 Mo1 12.5(2) . .
O3 Mo2 O7 Mo1 89.9(2) 2_655 .
V1 Mo2 O7 Mo1 53.58(14) . .
O8 Mo2 O7 Mo3 65.5(13) . .
O12 Mo2 O7 Mo3 -94.5(2) . .
O9 Mo2 O7 Mo3 2.8(2) . .
O2 Mo2 O7 Mo3 101.4(2) . .
O3 Mo2 O7 Mo3 178.8(2) 2_655 .
V1 Mo2 O7 Mo3 142.48(16) . .
O4 Mo1 O7 As1 153.2(13) . .
O5 Mo1 O7 As1 -37.7(4) . .
O6 Mo1 O7 As1 -135.6(4) . .
O2 Mo1 O7 As1 125.1(4) . .
O3 Mo1 O7 As1 48.0(4) . .
V1 Mo1 O7 As1 84.3(3) . .
O4 Mo1 O7 Mo2 15.4(15) . .
O5 Mo1 O7 Mo2 -175.5(2) . .
O6 Mo1 O7 Mo2 86.7(3) . .
O2 Mo1 O7 Mo2 -12.6(2) . .
O3 Mo1 O7 Mo2 -89.8(2) . .
V1 Mo1 O7 Mo2 -53.47(14) . .
O4 Mo1 O7 Mo3 -74.2(15) . .
O5 Mo1 O7 Mo3 94.9(2) . .
O6 Mo1 O7 Mo3 -3.0(2) . .
O2 Mo1 O7 Mo3 -102.3(2) . .
O3 Mo1 O7 Mo3 -179.4(2) . .
V1 Mo1 O7 Mo3 -143.11(16) . .
O10 Mo3 O7 As1 -180(100) . .
O11 Mo3 O7 As1 42.5(3) . .
O14 Mo3 O7 As1 -43.0(3) . .
O9 Mo3 O7 As1 -134.4(4) . .
O6 Mo3 O7 As1 134.7(4) . .
O10 Mo3 O7 Mo2 -48.1(15) . .
O11 Mo3 O7 Mo2 174.2(2) . .
O14 Mo3 O7 Mo2 88.7(2) . .
O9 Mo3 O7 Mo2 -2.7(2) . .
O6 Mo3 O7 Mo2 -93.6(2) . .
O10 Mo3 O7 Mo1 48.3(15) . .
O11 Mo3 O7 Mo1 -89.4(2) . .
O14 Mo3 O7 Mo1 -174.9(2) . .
O9 Mo3 O7 Mo1 93.7(2) . .
O6 Mo3 O7 Mo1 2.8(2) . .
O8 Mo2 O9 Mo3 -172.9(4) . .
O12 Mo2 O9 Mo3 81.4(4) . .
O2 Mo2 O9 Mo3 -72.0(4) . .
O3 Mo2 O9 Mo3 -15.0(9) 2_655 .
O7 Mo2 O9 Mo3 -4.3(3) . .
V1 Mo2 O9 Mo3 -58.3(4) . .
O10 Mo3 O9 Mo2 176.5(4) . .
O11 Mo3 O9 Mo2 -2.8(8) . .
O14 Mo3 O9 Mo2 -79.2(4) . .
O6 Mo3 O9 Mo2 76.5(4) . .
O7 Mo3 O9 Mo2 4.3(3) . .
O10 Mo3 O11 Mo6 133.8(8) . 2_655
O14 Mo3 O11 Mo6 30.5(8) . 2_655
O9 Mo3 O11 Mo6 -46.8(12) . 2_655
O6 Mo3 O11 Mo6 -125.1(9) . 2_655
O7 Mo3 O11 Mo6 -53.6(8) . 2_655
O8 Mo2 O12 Mo5 132.6(8) . .
O9 Mo2 O12 Mo5 -125.0(8) . .
O2 Mo2 O12 Mo5 -18.5(12) . .
O3 Mo2 O12 Mo5 32.8(8) 2_655 .
O7 Mo2 O12 Mo5 -51.8(8) . .
V1 Mo2 O12 Mo5 19.3(9) . .
O17 Mo5 O12 Mo2 -133.7(8) . .
O5 Mo5 O12 Mo2 -31.3(8) 2_655 .
O16 Mo5 O12 Mo2 48.6(12) . .
O15 Mo5 O12 Mo2 124.7(8) . .
O13 Mo5 O12 Mo2 53.1(8) . .
O13 As1 O13 Mo4 63.4(3) 2_655 .
O7 As1 O13 Mo4 -177.0(3) 2_655 .
O7 As1 O13 Mo4 -56.2(4) . .
O13 As1 O13 Mo5 -179.7(4) 2_655 .
O7 As1 O13 Mo5 -60.0(4) 2_655 .
O7 As1 O13 Mo5 60.7(4) . .
O13 As1 O13 Mo6 -63.2(3) 2_655 .
O7 As1 O13 Mo6 56.4(4) 2_655 .
O7 As1 O13 Mo6 177.1(3) . .
O21 Mo4 O13 As1 -152.4(11) . .
O14 Mo4 O13 As1 38.1(4) . .
O15 Mo4 O13 As1 136.0(4) . .
O19 Mo4 O13 As1 -125.5(4) . .
O20 Mo4 O13 As1 -48.2(3) 2_655 .
V2 Mo4 O13 As1 -84.5(3) . .
O21 Mo4 O13 Mo5 74.6(13) . .
O14 Mo4 O13 Mo5 -94.9(2) . .
O15 Mo4 O13 Mo5 3.0(2) . .
O19 Mo4 O13 Mo5 101.5(2) . .
O20 Mo4 O13 Mo5 178.8(2) 2_655 .
V2 Mo4 O13 Mo5 142.49(16) . .
O21 Mo4 O13 Mo6 -14.6(13) . .
O14 Mo4 O13 Mo6 175.9(2) . .
O15 Mo4 O13 Mo6 -86.2(2) . .
O19 Mo4 O13 Mo6 12.35(19) . .
O20 Mo4 O13 Mo6 89.6(2) 2_655 .
V2 Mo4 O13 Mo6 53.34(13) . .
O17 Mo5 O13 As1 -178.0(17) . .
O5 Mo5 O13 As1 42.4(3) 2_655 .
O12 Mo5 O13 As1 -43.3(3) . .
O16 Mo5 O13 As1 134.8(4) . .
O15 Mo5 O13 As1 -134.8(4) . .
O17 Mo5 O13 Mo4 -46.1(18) . .
O5 Mo5 O13 Mo4 174.3(2) 2_655 .
O12 Mo5 O13 Mo4 88.7(2) . .
O16 Mo5 O13 Mo4 -93.2(2) . .
O15 Mo5 O13 Mo4 -2.8(2) . .
O17 Mo5 O13 Mo6 50.2(18) . .
O5 Mo5 O13 Mo6 -89.5(2) 2_655 .
O12 Mo5 O13 Mo6 -175.1(2) . .
O16 Mo5 O13 Mo6 3.0(2) . .
O15 Mo5 O13 Mo6 93.4(2) . .
O18 Mo6 O13 As1 150.1(11) . .
O11 Mo6 O13 As1 -38.4(4) 2_655 .
O16 Mo6 O13 As1 -135.9(4) . .
O20 Mo6 O13 As1 48.0(3) . .
O19 Mo6 O13 As1 125.3(4) . .
O18 Mo6 O13 Mo4 12.4(13) . .
O11 Mo6 O13 Mo4 -176.1(2) 2_655 .
O16 Mo6 O13 Mo4 86.4(2) . .
O20 Mo6 O13 Mo4 -89.7(2) . .
O19 Mo6 O13 Mo4 -12.4(2) . .
O18 Mo6 O13 Mo5 -77.2(12) . .
O11 Mo6 O13 Mo5 94.4(2) 2_655 .
O16 Mo6 O13 Mo5 -3.1(2) . .
O20 Mo6 O13 Mo5 -179.2(2) . .
O19 Mo6 O13 Mo5 -101.9(2) . .
O21 Mo4 O14 Mo3 130.5(8) . .
O15 Mo4 O14 Mo3 -125.2(8) . .
O19 Mo4 O14 Mo3 -17.3(12) . .
O20 Mo4 O14 Mo3 31.7(8) 2_655 .
O13 Mo4 O14 Mo3 -51.7(8) . .
V2 Mo4 O14 Mo3 19.6(9) . .
O10 Mo3 O14 Mo4 -134.6(8) . .
O11 Mo3 O14 Mo4 -31.2(8) . .
O9 Mo3 O14 Mo4 124.1(8) . .
O6 Mo3 O14 Mo4 47.8(12) . .
O7 Mo3 O14 Mo4 53.0(8) . .
O21 Mo4 O15 Mo5 -172.9(4) . .
O14 Mo4 O15 Mo5 81.1(4) . .
O19 Mo4 O15 Mo5 -72.4(4) . .
O20 Mo4 O15 Mo5 -15.1(9) 2_655 .
O13 Mo4 O15 Mo5 -4.4(3) . .
V2 Mo4 O15 Mo5 -58.9(4) . .
O17 Mo5 O15 Mo4 177.9(4) . .
O5 Mo5 O15 Mo4 -2.4(9) 2_655 .
O12 Mo5 O15 Mo4 -79.6(4) . .
O16 Mo5 O15 Mo4 77.3(4) . .
O13 Mo5 O15 Mo4 4.5(3) . .
O18 Mo6 O16 Mo5 172.7(4) . .
O11 Mo6 O16 Mo5 -80.5(4) 2_655 .
O20 Mo6 O16 Mo5 14.7(9) . .
O19 Mo6 O16 Mo5 72.6(4) . .
O13 Mo6 O16 Mo5 4.6(3) . .
O17 Mo5 O16 Mo6 -177.6(4) . .
O5 Mo5 O16 Mo6 78.8(4) 2_655 .
O12 Mo5 O16 Mo6 0.1(9) . .
O15 Mo5 O16 Mo6 -77.1(4) . .
O13 Mo5 O16 Mo6 -4.7(3) . .
O22 V2 O19 Mo6 -117.60(18) . .
O20 V2 O19 Mo6 120.8(3) 2_655 .
O20 V2 O19 Mo6 3.7(2) . .
O19 V2 O19 Mo6 62.40(18) 2_655 .
Mo6 V2 O19 Mo6 101.97(19) 2_655 .
Mo4 V2 O19 Mo6 124.6(3) . .
Mo4 V2 O19 Mo6 22.8(3) 2_655 .
O22 V2 O19 Mo4 117.81(17) . .
O20 V2 O19 Mo4 -3.8(2) 2_655 .
O20 V2 O19 Mo4 -120.8(3) . .
O19 V2 O19 Mo4 -62.18(18) 2_655 .
Mo6 V2 O19 Mo4 -22.6(3) 2_655 .
Mo4 V2 O19 Mo4 -101.8(2) 2_655 .
O18 Mo6 O19 V2 93.7(3) . .
O11 Mo6 O19 V2 -55.2(6) 2_655 .
O16 Mo6 O19 V2 -163.5(3) . .
O20 Mo6 O19 V2 -3.5(2) . .
O13 Mo6 O19 V2 -91.5(2) . .
O18 Mo6 O19 Mo4 -157.9(3) . .
O11 Mo6 O19 Mo4 53.3(7) 2_655 .
O16 Mo6 O19 Mo4 -55.0(3) . .
O20 Mo6 O19 Mo4 104.9(3) . .
O13 Mo6 O19 Mo4 17.0(3) . .
O21 Mo4 O19 V2 -93.8(3) . .
O14 Mo4 O19 V2 54.5(6) . .
O15 Mo4 O19 V2 163.5(3) . .
O20 Mo4 O19 V2 3.5(2) 2_655 .
O13 Mo4 O19 V2 91.6(2) . .
O21 Mo4 O19 Mo6 157.6(3) . .
O14 Mo4 O19 Mo6 -54.1(7) . .
O15 Mo4 O19 Mo6 54.9(3) . .
O20 Mo4 O19 Mo6 -105.1(3) 2_655 .
O13 Mo4 O19 Mo6 -17.0(3) . .
V2 Mo4 O19 Mo6 -108.6(4) . .
O22 V2 O20 Mo6 101.4(2) . .
O20 V2 O20 Mo6 -78.6(2) 2_655 .
O19 V2 O20 Mo6 -152.9(3) 2_655 .
O19 V2 O20 Mo6 -3.8(2) . .
Mo6 V2 O20 Mo6 -118.3(2) 2_655 .
Mo4 V2 O20 Mo6 -38.5(2) . .
Mo4 V2 O20 Mo6 -156.7(4) 2_655 .
O22 V2 O20 Mo4 -101.9(2) . 2_655
O20 V2 O20 Mo4 78.1(2) 2_655 2_655
O19 V2 O20 Mo4 3.8(2) 2_655 2_655
O19 V2 O20 Mo4 152.9(3) . 2_655
Mo6 V2 O20 Mo4 38.4(2) 2_655 2_655
Mo4 V2 O20 Mo4 118.1(2) . 2_655
O18 Mo6 O20 V2 -93.6(3) . .
O11 Mo6 O20 V2 161.9(3) 2_655 .
O16 Mo6 O20 V2 64.6(7) . .
O19 Mo6 O20 V2 3.8(2) . .
O13 Mo6 O20 V2 74.3(3) . .
O18 Mo6 O20 Mo4 127.7(5) . 2_655
O11 Mo6 O20 Mo4 23.2(5) 2_655 2_655
O16 Mo6 O20 Mo4 -74.1(8) . 2_655
O19 Mo6 O20 Mo4 -135.0(6) . 2_655
O13 Mo6 O20 Mo4 -64.4(5) . 2_655
